Li~20~Mg~6~Cu~13~Al~42~: a new ordered quaternary superstructure to the icosahedral <i>T</i>-Mg~32~(Zn,Al)~49~ phase with fullerene-like Al~60~ cluster
Pavlyuk, Nazar; Dmytriv, Grygoriy; Pavlyuk, Volodymyr; Ehrenberg, Helmut; Acta Crystallographica Section B 75 (2019) –; doi:10.1107/S2052520619000349

data_2108379
_publ_section_title
;
 Li~20~Mg~6~Cu~13~Al~42~: a new ordered quaternary superstructure to the
 icosahedral <i>T</i>-Mg~32~(Zn,Al)~49~ phase with fullerene-like Al~60~
 cluster
;
_journal_coeditor_code           RA5047
_journal_issue                   2
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first
;
;
_journal_paper_doi               10.1107/S2052520619000349
_journal_volume                  75
_journal_year                    2019
_chemical_formula_sum            'Al84 Cu26 Li40 Mg12'
_chemical_formula_weight         4487.68
_space_group_crystal_system      cubic
_space_group_IT_number           204
_space_group_name_Hall           '-I 2 2 3'
_space_group_name_H-M_alt        'I m -3'
_symmetry_space_group_name_Hall  '-I 2 2 3'
_symmetry_space_group_name_H-M   'I m -3'
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   13.8451(2)
_cell_length_b                   13.8451(2)
_cell_length_c                   13.8451(2)
_cell_measurement_reflns_used    495
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.517
_cell_measurement_theta_min      2.080
_cell_volume                     2653.92(7)
_computing_cell_refinement       'CrysAlis CCD (Oxford Diffraction, 2008)'
_computing_data_collection       'CrysAlis CCD (Oxford Diffraction, 2008)'
_computing_data_reduction        'CrysAlis RED (Oxford Diffraction, 2008)'
_computing_molecular_graphics    'DIAMOND (Brandenburg, 2006)'
_computing_publication_material  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXS-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.991
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measurement_device_type  'Oxford Diffraction Xcalibur3 CCD'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0220
_diffrn_reflns_av_unetI/netI     0.0393
_diffrn_reflns_Laue_measured_fraction_full 0.991
_diffrn_reflns_Laue_measured_fraction_max 0.993
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            3444
_diffrn_reflns_point_group_measured_fraction_full 0.991
_diffrn_reflns_point_group_measured_fraction_max 0.993
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.517
_diffrn_reflns_theta_min         2.080
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    5.878
_exptl_absorpt_correction_T_max  0.785
_exptl_absorpt_correction_T_min  0.662
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details   '(CrysAlis RED; Oxford Diffraction, 2008)'
_exptl_crystal_colour            'metallic grey'
_exptl_crystal_density_diffrn    2.808
_exptl_crystal_density_meas      2.81(3)
_exptl_crystal_density_method    volumetric
_exptl_crystal_description       prism
_exptl_crystal_F_000             2110
_exptl_crystal_size_max          0.07
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.04
_refine_diff_density_max         0.534
_refine_diff_density_min         -0.481
_refine_diff_density_rms         0.147
_refine_ls_extinction_coef       0.00138(13)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.040
_refine_ls_matrix_type           full
_refine_ls_number_parameters     42
_refine_ls_number_reflns         574
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.040
_refine_ls_R_factor_all          0.0241
_refine_ls_R_factor_gt           0.0231
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0235P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0618
_refine_ls_wR_factor_ref         0.0619
_reflns_Friedel_coverage         0.000
_reflns_number_gt                495
_reflns_number_total             574
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            ra5047Isup1.cif
_cod_data_source_block           I
_cod_original_cell_volume        2653.92(12)
_cod_database_code               2108379
_shelx_shelxl_version_number     2014/7
_shelx_res_checksum              56692
_shelx_hkl_checksum              36502
_cod_database_fobs_code 2108379